Compression of Silver Sulfide: X-ray Diffraction Measurements and Total-Energy Calculations
David Santamaría-Pérez; Miriam Marqués; Raquel Chuliá-Jordán; José Manuel Menendez; Oscar Gomis; Javier Ruiz-Fuertes; Juan Antonio Sans; Daniel Errandonea; José Manuel Recio; Inorganic Chemistry 51 (2012) 5289–5298; doi:10.1021/ic300236p

data_4329109
_publ_contact_author_address
; 
Departamento de Quimica-Fisica I
Universidad Complutense de Madrid
Avda Complutense s/n, E-28040, Madrid
Spain
;
_publ_contact_author_email       dsantamaria@quim.ucm.es
_publ_contact_author_name        'Dr. David Santamaria-Perez'
_publ_contact_author_phone       0034913945206
_publ_section_title
;
 Compression of Silver Sulfide: X-ray Diffraction Measurements and
 Total-Energy Calculations
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5289
_journal_page_last               5298
_journal_paper_doi               10.1021/ic300236p
_journal_volume                  51
_journal_year                    2012
_chemical_formula_moiety         'Ag2 S'
_chemical_formula_sum            'Ag2 S'
_chemical_formula_weight         247.80
_chemical_name_common            'Silver sulfide'
_chemical_name_systematic        ' ?'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90.00000
_cell_angle_beta                 93.819(15)
_cell_angle_gamma                90.00000
_cell_formula_units_Z            4
_cell_length_a                   4.0920(8)
_cell_length_b                   5.7519(13)
_cell_length_c                   7.9702(17)
_cell_measurement_temperature    293
_cell_volume                     187.18(7)
_computing_structure_refinement  FULLPROF
_diffrn_ambient_temperature      293
_diffrn_detector                 CCD
_diffrn_detector_type            CCD
_diffrn_measurement_device_type  'Diamond I15 beamline'
_diffrn_radiation_type           'Synchrotron X-ray radiation'
_diffrn_radiation_wavelength     0.4246
_diffrn_source                   synchrotron
_pd_char_colour                  black
_pd_instr_location               ' Synchrotron radiation'
_pd_meas_2theta_range_inc        0.014277
_pd_meas_2theta_range_max        21.40637
_pd_meas_2theta_range_min        2.48944
_pd_meas_number_of_points        1327
_pd_meas_scan_method             fixed
_pd_proc_2theta_range_inc        0.014277
_pd_proc_2theta_range_max        21.4064
_pd_proc_2theta_range_min        2.4894
_pd_proc_ls_background_function  '32 background points'
_pd_proc_ls_pref_orient_corr     ' ?'
_pd_proc_ls_profile_function     pseudo-Voigt
_pd_proc_ls_prof_R_factor        0.134642
_pd_proc_ls_prof_wR_expected     0.052088
_pd_proc_ls_prof_wR_factor       0.191287
_pd_proc_wavelength              0.424596
_pd_spec_mounting                ' Diamond-anvil cell (DAC) '
_pd_spec_mount_mode              transmission
_pd_spec_shape                   cylinder
_pd_spec_size_axial              0.2
_pd_spec_size_equat              0.05
_refine_ls_number_parameters     19
_refine_ls_number_reflns         171
_refine_ls_number_restraints     0
_refine_ls_R_I_factor            0.037249
_cod_data_source_file            ic300236p_si_001_3.cif
_cod_data_source_block           phase3
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               4329109
_pd_proc_ls_prof_cr_factor       0.094709
_pd_proc_ls_prof_cwr_factor      0.089399
_pd_proc_ls_prof_cwr_expected    0.024344
_pd_proc_ls_prof_chi2            13.4863
_pd_proc_ls_prof_echi2           14.1119